Modeling Materials and Processes in Hybrid/Organic Photovoltaics: From Dye-Sensitized to Perovskite Solar Cells Filippo De Angelis* Computational Laboratory for Hybrid/Organic Photovoltaics (CLHYO), CNR-ISTM, Via Elce di Sotto 8, 06123 Perugia, Italy S Supporting Information *
CONSPECTUS: Over the last 2 decades, researchers have invested enormous research eﬀort into hybrid/organic photovoltaics, leading to the recent launch of the ﬁrst commercial products that use this technology. Dye-sensitized solar cells (DSCs) have shown clear advantages over competing technologies. The top certiﬁed eﬃciency of DSCs exceeds 11%, and the laboratory-cell eﬃciency is greater than 13%. In 2012, the ﬁrst reports of high eﬃciency solid-state DSCs based on organohalide lead perovskites completely revolutionized the ﬁeld. These materials are used as light absorbers in DSCs and as light-harvesting materials and electron conductors in meso-superstructured and ﬂat heterojunction solar cells and show certiﬁed eﬃciencies that exceed 17%. To eﬀectively compete with conventional photovoltaics, emerging technologies such as DSCs need to achieve higher eﬃciency and stability, while maintaining low production costs. Many of the advances in the DSC ﬁeld have relied on the computational design and screening of new materials, with researchers examining material characteristics that can improve device performance or stability. Suitable modeling strategies allow researchers to observe the otherwise inaccessible but crucial heterointerfaces that control the operation of DSCs, oﬀering the opportunity to develop new and more eﬃcient materials and optimize processes. In this Account, we present a uniﬁed view of recent computational modeling research examining DSCs, illustrating how the principles and simulation tools used for these systems can also be adapted to study the emerging ﬁeld of perovskite solar cells. Researchers have widely applied ﬁrst-principles modeling to the DSC ﬁeld and, more recently, to perovskite-based solar cells. DFT/TDDFT methods provide the basic framework to describe most of the desired materials and interfacial properties, and Car−Parrinello molecular dynamics allow researchers the further ability to sample local minima and dynamical ﬂuctuations at ﬁnite temperatures. However, conventional DFT/TDDFT has some limitations, which can be overcome in part by tailored solutions or using many body perturbation theory within the GW approach, which is however more computationally intensive. Relativistic eﬀects, such as spin−orbit coupling, are also included in simulations since they are fundamental for addressing systems that contain heavy atoms. We illustrate the performance of the proposed simulation toolbox along with the fundamental modeling strategies using selected examples of relevant isolated device constituents, including dye and perovskite absorbers, metal-oxide surfaces and nanoparticles, and hole transporters. We critically assess the accuracy of various computational approaches against the related experimental data. We analyze the representative interfaces that control the operational mechanism of the devices, including dye-sensitized TiO2/hole transporter and organohalide lead perovskite/TiO2, and the results reveal fundamental aspects of the device’s operational mechanism. Although the modeling of DSCs is relatively mature, the recent “perovskite storm” has presented new problems and new modeling challenges, such as understanding exciton formation and dissociation at interfaces and carrier recombination in these materials.
oxide surface is a monolayer of sensitizing dye, which absorbs the solar radiation and injects photoexcited electrons into the semiconductor conduction band (CB). The oxidized dye is reduced by the hole transporter, which is in turn reduced at the counter-electrode, closing the circuit. The highest DSC eﬃciency has been obtained with a liquid hole transporter, I−/I3− or Co(II)/Co(III) redox couples in organic solvents.
Solar technologies, in particular photovoltaics, are foreseen as a major source of renewable energy. Hybrid/organic photovoltaics has witnessed a huge research eﬀort in the last 2 decades, recently leading to the ﬁrst commercial products. Dyesensitized solar cells (DSCs)1 have maintained a clear lead in eﬃciency and stability over competitive technologies, with top certiﬁed eﬃciency exceeding 11% and laboratory-cell eﬃciency above 13%.2 Crucial to functioning of the DSCs is the photoinduced charge separation occurring at the heterointerface(s) between a sensitized metal-oxide electrode, typically TiO2, and a hole transporter (HT), Scheme 1a. Grafted on the © XXXX American Chemical Society
Special Issue: DFT Elucidation of Materials Properties Received: February 28, 2014
dx.doi.org/10.1021/ar500089n | Acc. Chem. Res. XXXX, XXX, XXX−XXX
Accounts of Chemical Research
Scheme 1. Energy Levels and Schematic Operational Mechanism of (a) DSCs, (b) perovskite based DSCs (TiO2) or MSSCs (Al2O3), and (c) Perovskite Flat Heterojunctiona
The TiO2 DOS is represented by gray and the perovskite DOS by red areas.
The ﬁeld has been completely revolutionized in 2012 by the ﬁrst reports of high eﬃciency solid-state DSCs based on organohalide perovskites (e.g., methylammonium lead iodide, MAPbI3) as light absorbers,3 Scheme 1b, which led to 15% eﬃciency.4 Lee et al.5 further demonstrated that a similar perovskite can serve both as light harvesting material and as electron conductor in meso-superstructured solar cells (MSSCs), currently exceeding 15% eﬃciency. These devices, in which TiO2 was replaced by an insulating Al2O3 scaﬀold, represent a new generation of photovoltaic devices. The ﬁeld further evolved toward a planar heterojunction incorporating a vapor-deposited perovskite, Scheme 1c, which exceeded 15% eﬃciency.6 First-principles modeling has been widely applied to the DSC ﬁeld7−10 and more recently to perovskite-based solar cells.11−13 On the one hand, one wishes to design and screen new materials, with tailored and engineered characteristics for improved device performance and stability. On the other hand, modeling may oﬀer a hitherto inaccessible view of the heterointerfaces ruling the device operational mechanism. To eﬀectively compete with existing photovoltaics, emerging technologies need to achieve high eﬃciency and stability, maintaining low production costs. The solar cell eﬃciency (η) is deﬁned as η=
A computational approach to hybrid/organic photovoltaics can be cast into a stepwise problem, whereby one needs to accurately simulate the individual components, to move to the relevant heterointerfaces. The fundamental information required on individual materials is (i) the absorber structures, energy levels, and optical absorption spectra, (ii) a model for the metal-oxide surface, along with its CB energy and density of states, and (iii) the hole-transporter oxidation potential. This information constitutes the basis for the design and screening of new materials, and thus a fast and eﬀective computational tool is required. For the interacting absorber/metal oxide/hole transporter, one needs to calculate (i) the interface structure and (ii) the nature/localization of excited states and the energy level alignment. An alternative strategy, not discussed here, is the explicit simulation of photoinduced electron transfers relevant to DSCs by quantum or nonadiabatic dynamics.8,15 Density functional theory (DFT) and time-dependent DFT (TDDFT) provide the framework to describe most of the desired materials and interfacial properties. DFT-based Car− Parrinello molecular dynamics14 further allows us to sample the investigated systems at ﬁnite temperature. Conventional DFT/ TDDFT have however some limitations in the description of dispersion interactions, of semiconductor band gaps, and of charge-transfer excited states; thus speciﬁcally tailored DFT approaches can be adopted. Many body perturbation theory, within the GW approach, constitutes a solid framework to improve upon DFT. GW is however (much) more computationally demanding than DFT, limiting its routine application. A general issue with all computational tools is the inclusion of relativistic eﬀects. These are usually approximated by scalarrelativistic (SR) and, to higher order, by spin−orbit coupling (SOC) contributions, and they cannot be neglected in heavyelement-containing systems. In this Account, I oﬀer a uniﬁed view of recent activity in the computational modeling of DSCs, illustrating how the same principles and simulation tools, properly adapted, can be employed in the emerging ﬁeld of perovskite solar cells. The challenges and unsolved issues are highlighted.
Jsc Voc FF PI
where Jsc is the photocurrent density at short circuit, FF is the cell ﬁll factor, PI is the intensity of the incident light, and Voc is the open circuit voltage of the cell, whose deﬁnition in terms of energy levels varies with the type of device, Scheme 1. J sc is the integral over the solar spectrum of the monochromatic incident photon-to-current conversion eﬃciency (IPCE) under short circuit conditions, and as such it depends directly on the absorber. The DSCs Voc represents the diﬀerence between the quasi-Fermi level of the metal oxide under illumination and the hole transporter redox potential, Scheme 1a, the latter being nearly constant. In DSCs, Voc depends only indirectly on the absorber, while the absorber CB energy ﬁxes the device V oc in MSSCs and in ﬂat heterojunctions, Scheme 1b,c. The FF is an adimensional parameter that reﬂects the shape of the J−V curve. B
dx.doi.org/10.1021/ar500089n | Acc. Chem. Res. XXXX, XXX, XXX−XXX
Accounts of Chemical Research
Figure 1. Calculated structures of selected ruthenium (top) and organic dyes (bottom).
2. MODELING INDIVIDUAL DEVICE COMPONENTS
Most notably, the investigated ruthenium dyes, for example, N3 or black dye, were nicely calculated without inclusion of relativistic eﬀects. Signiﬁcantly, however, the enhanced DX1 spectral response was attributed to SOC-promoted spinforbidden transitions.17 The electronic and optical properties of the panchromatic black dye and DX1 dyes were thus investigated by SR- and SOC-TDDFT,21,22 employing B3LYP and a continuum solvation model, see Figure 2a,b for a comparison between simulated and experimental spectra. The room-temperature spectra of black dye and DX1 are nicely reproduced by both SR- and SOC-TDDFT, the latter introducing only a slight spectral broadening in the lower energy range. Also, the energy of the lowest dye excited state, relevant to set the energetics of electron injection onto TiO2, is marginally aﬀected by SOC. To further quantify the impact of SOC, we compared our calculations with the low-temperature DX1 absorption spectrum. Figure 2c highlights two excitations originated by mixing of the lowest singlet excited state with low-lying triplet excitations. The calculated molar extinction coeﬃcient of DX1, 2988 M−1 cm−1 at 1.58 eV, is in excellent agreement with the ∼3000 M−1 cm−1 experimental value. We thus estimated the impact of SOC on the IPCE and Jsc generation due to the lowest absorption band (from 1.3 to 1.9 eV), Figure 2d. Assuming a 0.5 M dye concentration, a 10 μm ﬁlm thickness, and a unitary injection and collection eﬃciency, we can calculate IPCE(λ).21 The results highlight how SOC contributes an overall Jsc gain of 2.3 mA/cm2 in the
2.1. Dye Sensitizers
Ru(II)−polypyridyl complexes, such as the N3, N719,16 and black dye, Figure 1, had a central role in advancing DSC technology. A novel black-dye-like trans-dichloro-Ru(II) dye was recently reported,17 DX1 in Figure 1, which showed enhanced spectral response in the 700−900 nm region allowing demonstration of a record Jsc. Fully organic push−pull sensitizers, Figure 1, have been developed because of their increased molar extinction coeﬃcient, spectral tunability, and reduced environmental impact. Functionalized donor−acceptor Zn(II)-porphyrins have more recently emerged as a new class of sensitizers with high performance, due to their extended absorption spectrum.2 Standard DFT/TDDFT including solvation eﬀects proved to be extremely successful in reproducing the electronic and optical properties of ruthenium dyes, Figure 2a,b;18,19 the ground and excited state oxidation potentials of the N3/N719 dyes were calculated within